Hydration and Durability of Concrete Containing Supplementary Cementitious Materials
View this Special IssueResearch Article  Open Access
Wonsuk Jung, SeJin Choi, "Effect of HighTemperature Curing Methods on the Compressive Strength Development of Concrete Containing High Volumes of Ground Granulated BlastFurnace Slag", Advances in Materials Science and Engineering, vol. 2017, Article ID 7210591, 6 pages, 2017. https://doi.org/10.1155/2017/7210591
Effect of HighTemperature Curing Methods on the Compressive Strength Development of Concrete Containing High Volumes of Ground Granulated BlastFurnace Slag
Abstract
This paper investigates the effect of the hightemperature curing methods on the compressive strength of concrete containing high volumes of ground granulated blastfurnace slag (GGBS). GGBS was used to replace Portland cement at a replacement ratio of 60% by binder mass. The hightemperature curing parameters used in this study were the delay period, temperature rise, peak temperature (PT), peak period, and temperature down. Test results demonstrate that the compressive strength of the samples with PTs of 65°C and 75°C was about 88% higher than that of the samples with a PT of 55°C after 1 day. According to this investigation, there might be optimum hightemperature curing conditions for preparing a concrete containing high volumes of GGBS, and incorporating GGBS into precast concrete mixes can be a very effective tool in increasing the applicability of this byproduct.
1. Introduction
About 14 million tons of blastfurnace slag, the byproduct of steel industry, is produced annually in Korea [1]. Ground granulated blastfurnace slag (GGBS), either as a constituent of cement or as a mineral admixture, is widely used to make not only traditional concrete but also highperformance concrete, which has several advantages including workability, longterm strength, and durability [2]. Recently, to reduce CO_{2} production in the cement and concrete industry, many studies have been conducted on environmentally friendly concrete with highvolume supplementary cementitious materials [3–9]. It was reported [10–12] that concrete using GGBS has the advantage of an earlier strength development under hightemperature curing conditions owing to the temperaturedependent characteristic of GGBS. Owing to this, GGBS might be effectively used in preparing precast concrete manufactured with hightemperature curing.
While significant literature is available on supplementary cementitious materials in concrete, such as GGBS and fly ash, few works have studied the effect of hightemperature curing conditions on the strength properties of concrete containing highvolume supplementary cementitious materials [11, 13–15]. Miura and Iwaki [11] evaluated the strength development of concrete incorporating high levels of GGBS at low temperatures, demonstrating that GGBS concrete with a specific surface area of 400 m^{2}/kg faces serious strength development problems at early ages and with low curing temperatures. Aldea et al. [13] investigated the effects of curing conditions on the properties of concrete prepared with slag replacement. Test results indicated that slag replacement of up to 50% by mass had little effect on strength and steam curing reduced the compressive strength as compared to other curing types (such as autoclaving and normal curing). Yazici et al. [14] investigated the effect of steam curing on class C highvolume fly ash concrete mixtures, indicating that steam curing accelerated the 1day strength development but the longterm strength was greatly reduced. Liu et al. [15] evaluated the influence of steam curing on the compressive strength of concrete containing supplementary cementing materials. Test results indicated that the concrete containing ultrafine fly ash (UFA) had a low early strength after 13 hours of steam curing and the difference between the 28day compressive strength of 13hour steamcured concrete and that of moistcured concrete was large.
This study examines how the compressive strength of concrete containing high volumes of GGBS is affected by various hightemperature curing methods. To date, the compressive strength development of highvolume GGBS concrete according to various hightemperature curing conditions—including delay period, temperature rise, peak temperature and period, and temperature down—has not been reported. The goal of this work is to demonstrate how GGBS can be used more efficiently and effectively in precast concrete using hightemperature curing methods.
2. Materials and Methods
2.1. Materials
ASTM Type I Portland cement with a specific gravity of 3.15 and crushed gravel with a specific gravity of 2.67 and fineness modulus of 6.75 were used. The fine aggregates used were crushed sand and washed sea sand (specific gravities of 2.62 and 2.66, resp.), which are commonly used in Korea. GGBS with a specific gravity of 2.89 and Blaine fineness of 4490 cm^{2}/g was obtained from Pohang, South Korea. The chemical composition of the cement and GGBS, determined by Xray fluorescence, is shown in Table 1.

2.2. Mix Proportions and Specimen Preparation
In this study, GGBS was used to replace Portland cement at a replacement ratio of 60% by binder mass. A constant watertobinder ratio (w/b) of 0.35 was used in this investigation. The mix proportions are given in Table 2.

Concrete was mixed in a twin shaft mechanical mixer. Specimens were cast in a cylindrical mold (100 mm diameter, 200 mm length) for the compressive strength test. After casting, the cylinder molds were moved to the autotemperaturecontrolled curing chamber with a 100% relative humidity, shown in Figure 1, and cured according to various hightemperature curing methods. The samples were then removed from the molds and cured in a watercuring tank before the compressive strength test.
Figure 2 shows the common hightemperature curing cycle used in manufacturing precast concrete. The hightemperature curing methods used in this investigation involved delay periods (DPs) of 2, 3, and 4 h at 20°C; temperature rises (TRs) of 10, 15, and 20°C/h; peak temperatures (PTs) of 55, 65, and 75°C; peak periods (PPs) of 3, 4, and 5 h; and temperature downs (TDs) of 5, 10, and 15°C/h. The hightemperature curing methods are detailed in Figure 3 and Table 3. The compressive strength of the concrete was tested after 1, 14, and 28 days, in accordance with ASTM C39. Each strength is the average value of three samples.

(a) Delay period condition
(b) Temperature rise condition
(c) Peak temperature condition
(d) Peak period condition
(e) Temperature down condition
3. Results and Discussion
3.1. Delay Period and Compressive Strength
The variation in the compressive strength with DP is shown in Figure 4. The 1day compressive strength of concrete mixes with DPs of 2, 3, and 4 h was 30, 32.5, and 31 MPa, respectively. After 14 days, the values for the mixes with a DP of 3 h were about 4.8–8.8% higher than the other mixes. In addition, the compressive strength of the concrete mix with a DP of 3 h was greater than the other mixes after 28 days, with a value of 49.5 MPa. In contrast, the DP of 2 h gave the lowest values for each test day. After 28 days, the compressive strength of the 3 h DP concrete was about 10% higher than that with a DP of 2 h.
3.2. Temperature Rise and Compressive Strength
The compressive strength variation with TR is given in Figure 5 at different ages. The 1day compressive strength of the sample with a TR of 15°C/h was 32.5 MPa, and this value was higher than that of other samples with a compressive strength of 2728 MPa. The compressive strength of the 20°C/h TR concrete was 28 MPa after 1 day, about 3.7% higher than that for the 10°C/h TR concrete. However, the later compressive strength of the 20°C/h TR concrete was 41 MPa (14 days) and 47 MPa (28 days), about 2.1–5.0% lower than the corresponding values of 10°C/h TR sample. This test results demonstrate that high heating rate might result in an advantageous high early strength development, but a disadvantageous longterm strength development. An earlier study [11] reported that heat curing seems to have an adverse influence on strength development, particularly at later ages.
3.3. Peak Temperature and Compressive Strength
Figure 6 shows the compressive strength variation of concrete mixes with different PTs at different ages. The 1day compressive strength of the 65°C and 75°C PT samples was 32.5 and 32 MPa, respectively. These values are about 88–91% higher than that of the sample with the lowest PT of 55°C (17 MPa). This result is similar to that of a previous study [10]. Barnett et al. reported that the earlyage strength is much more sensitive to temperature for samples with higher levels of GGBS. The lowest 14day compressive strength was for the sample with a PT of 55°C (36 MPa). After 28 days, the compressive strength of the 65°C PT concrete was the greatest (49.5 MPa), being about 10–18% higher than the samples with PTs of 55°C and 75°C.
3.4. Peak Period and Compressive Strength
The variation in compressive strength with PP is given in Figure 7 for different ages. The 1day compressive strength was highest for the concrete with a PP of 4 h. The 1day compressive strength values of the samples with PPs of 3, 4, and 5 h were 25, 32.5, and 28 MPa, respectively. In addition, after 14 days, the compressive strength of the 4 h PP condition was 4.8% higher than that of the concrete with a PP of 3 h. After 28 days, the compressive strengths of all the samples were the same with values ranging from 49.5 to 50 MPa.
3.5. Temperature Down and Compressive Strength
Figure 8 shows the variation in the compressive strength for the concrete with different TD values at different ages. The 1day compressive strength of the concrete with a TD of 5°C/h (35 MPa) was about 30% higher than that with a TD of 15°C/h. It is assumed that the rapid cooling during steam curing might have a negative influence on the concrete compressive strength at an early age. The compressive strength of the 15°C/h TD condition was 40.5 MPa after 14 days, around 6–11% lower than the other mixes. However, the compressive strength of the concrete with a TD of 15°C/h was similar to that for the 10°C/h TD condition after 28 days.
4. Conclusions
The following conclusions were obtained from the present investigation.
(1) The compressive strength of the concrete mix with a DP of 3 h (49.5 MPa) was greater than that of the other mixes after 28 days. In contrast, the compressive strength of the mix with a DP of 2 h was the lowest value after 28 days.
(2) The compressive strength of the sample with a TR of 20°C/h was about 3.7% higher than that of the 10°C/h TR sample after 1 day. However, the compressive strength of the sample with 20°C/h TR was lower than that of the sample with a TR of 10°C/h. This demonstrates that the high heating rate might result in an advantageous high early strength development, but a disadvantageous longterm strength development.
(3) The 1day compressive strength of the samples with PTs of 65°C and 75°C was about 32 MPa, about 88% higher than the 55°C PT condition. After 28 days, the value for the sample with a PT of 65°C was the greatest.
(4) The compressive strength of the sample with a PP of 4 h was 4.8% higher than that of the 3 h PP sample after 14 days. After 28 days, the compressive strength of all the samples was the same.
(5) The 1day compressive strength of the sample with a TD of 5°C/h was about 30% higher than that with a TD of 15°C/h. It is assumed that the rapid cooling during steam curing might adversely affect the compressive strength of the concrete at an early age.
The results of this investigation suggest that there might be optimum hightemperature curing conditions for the preparation of concrete containing high volumes of GGBS. Incorporating GGBS into precast concrete mixes can be a very effective tool in reducing CO_{2} production in the cement industry and increasing the applicability of GGBS. Further studies are needed to establish the relationships between the strength properties of concrete containing high volumes of supplementary cementitious materials and the watertobinder ratio, mineral admixture type, and so on.
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.
Acknowledgments
This paper was supported by Wonkwang University in 2015.
References
 Korea Concrete Institute, “Concrete & Environment,” vol.2, Kimoondang, Seoul, Korea, 2016. View at: Google Scholar
 K. M. Lee, H. K. Lee, S. H. Lee, and G. Y. Kim, “Autogenous shrinkage of concrete containing granulated blastfurnace slag,” Cement and Concrete Research, vol. 36, no. 7, pp. 1279–1285, 2006. View at: Publisher Site  Google Scholar
 S.J. Choi and Y.S. Jeon, “The Fluidity and Hardened Properties of EcoFriendly Low Cement Concrete with 3 Types of Binders,” Journal of the Architectural Institute of Korea Structure & Construction, vol. 31, no. 11, pp. 63–70, 2015. View at: Publisher Site  Google Scholar
 H. Yazıcı, “The effect of curing conditions on compressive strength of ultra high strength concrete with high volume mineral admixtures,” Building and Environment, vol. 42, no. 5, pp. 2083–2089, 2007. View at: Publisher Site  Google Scholar
 M.H. Zhang and J. Islam, “Use of nanosilica to reduce setting time and increase early strength of concretes with high volumes of fly ash or slag,” Construction and Building Materials, vol. 29, no. 4, pp. 573–580, 2012. View at: Publisher Site  Google Scholar
 S.J. Choi, J.S. Mun, K.H. Yang, and S.J. Kim, “Compressive fatigue performance of fiberreinforced lightweight concrete with highvolume supplementary cementitious materials,” Cement and Concrete Composites, vol. 73, pp. 89–97, 2016. View at: Publisher Site  Google Scholar
 G. Hannesson, K. Kuder, R. Shogren, and D. Lehman, “The influence of high volume of fly ash and slag on the compressive strength of selfconsolidating concrete,” Construction and Building Materials, vol. 30, pp. 161–168, 2012. View at: Publisher Site  Google Scholar
 K. H. Mo, U. Johnson Alengaram, M. Z. Jumaat, and S. P. Yap, “Feasibility study of high volume slag as cement replacement for sustainable structural lightweight oil palm shell concrete,” Journal of Cleaner Production, vol. 91, pp. 297–304, 2015. View at: Publisher Site  Google Scholar
 I. Papayianni and E. Anastasiou, “Production of highstrength concrete using high volume of industrial byproducts,” Construction and Building Materials, vol. 24, no. 8, pp. 1412–1417, 2010. View at: Publisher Site  Google Scholar
 S. J. Barnett, M. N. Soutsos, S. G. Millard, and J. H. Bungey, “Strength development of mortars containing ground granulated blastfurnace slag: effect of curing temperature and determination of apparent activation energies,” Cement and Concrete Research, vol. 36, no. 3, pp. 434–440, 2006. View at: Publisher Site  Google Scholar
 T. Miura and I. Iwaki, “Strength development of concrete incorporating high levels of ground granulated blastfurnace slag at low temperature,” Materials Journal, vol. 97, no. 1, pp. 66–70, 2000. View at: Google Scholar
 J. I. Escalante, L. Y. Gómez, K. K. Johal, G. Mendoza, H. Mancha, and J. Méndez, “Reactivity of blastfurnace slag in Portland cement blends hydrated under different conditions,” Cement and Concrete Research, vol. 31, no. 10, pp. 1403–1409, 2001. View at: Publisher Site  Google Scholar
 C.M. Aldea, F. Young, K. Wang, and S. P. Shah, “Effects of curing conditions on properties of concrete using slag replacement,” Cement and Concrete Research, vol. 30, no. 3, pp. 465–472, 2000. View at: Publisher Site  Google Scholar
 H. Yazici, S. Aydin, H. Yiǧiter, and B. Baradan, “Effect of steam curing on class C highvolume fly ash concrete mixtures,” Cement and Concrete Research, vol. 35, no. 6, pp. 1122–1127, 2005. View at: Publisher Site  Google Scholar
 B. Liu, Y. Xie, and J. Li, “Influence of steam curing on the compressive strength of concrete containing supplementary cementing materials,” Cement and Concrete Research, vol. 35, no. 5, pp. 994–998, 2005. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2017 Wonsuk Jung and SeJin Choi. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.